# Technical Paper - On NC thermal decomposition

## Technical Paper - On NC thermal decomposition

**Technical Paper On NC thermal decomposition Mario Paquet Page 1 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Review of basic concepts related to the thermal decomposition of nitrocellulose Mario Paquet General Dynamics Ordnance and Tactical Systems - Canada Valleyfield 55 Masson Street, J6S 4V9 , Valleyfield, Qc, Canada Abstract There are 2 important shelf-lives of interest to nitrocellulose (NC) manufacturers and users: the time it will take under known non-isothermal storage conditions for the NC to fail the Methyl Violet Paper or Bergmann Junk stability tests and the time it will take for a NC to become a risk for storage or handling under similar thermal conditions. **

The paper presented as an EASSP technical paper (European Association for the Study of Safety Problems in the Production and Use of Propellants) reviews the behavior and characteristics of the self-heating chemicals in isothermal and non- isothermal mode and offer a simplified method to evaluate both shelf-lives. It provides a method to convert isothermal data to non-isothermal data. It also provides a rapid method for evaluating the remaining shelf-lives to stability test failure and to decomposition of NC samples in storage. The original EASSP paper included both NC and NG decomposition data and reviewed decomposition at atmospheric conditions and under pressure.

1 Introduction It is common, when working with nitrocellulose (NC), to use the NC decomposition temperature most often quoted in the literature and in Material Safety Data Sheet (MSDS) which is about 185°C. This is quite insufficient and misleading. In addition, most NC manufacturers and users have difficulty estimating the shelf-life of NC in storage under thermal conditions prevailing in various locations worldwide. The present paper reviews basic concepts related to the thermal decomposition of NC for the main purpose of providing a methodology that will enable NC manufacturers and users to establish approximated shelf-life of NC in storage.

It also proposes an empirical curve that enables the estimation of NC shelf-life under isothermal conditions and provides ways of calculating the equivalent shelf-life under non-isothermal conditions.

The reader must be warned that proper safety margins must be applied to these estimates as storage conditions cannot be known precisely and can be significantly heterogeneous, even if limited to one location. The approximations obtained are really order of magnitude estimates rather than precise finite evaluations. They provides sense for the time frame involved in NC decomposition in storage and may help in training plant personnel. Definition of various concepts related to Self-Heating Chemical under isothermal conditions The decomposition of NC under various isothermal conditions can be divided in 3 groups: -Fast decomposition (high temperatures), -Slow decomposition (low temperatures) -Transition between fast and slow decompositions (mid-range temperatures) Explosives are generally known as self-heating chemicals.

Self-heating chemicals can be divided in 2 main groups: The TD group and the AC group.

The Thermal Decomposition (TD) group Chemicals from the Thermal Decomposition (TD) group will be characterized by a Critical Temperature (Tc) above which the exothermic decomposition provides enough heat for the temperature to increase in the center of the mass even under isothermal conditions. At some point ignition will occur. For these chemicals, thermal decomposition is present at temperatures below the Tc however it is not energetic enough to cause the mass to self-heat. Tc is affected by the size and shape of the samples and for larger masses; lower Tc are expected. This is the case for coal dust, sawdust, oil rags and others which are of the TD type.

**Tc is usually estimated using the Semenov and/or the Frank-Kamenetskii equations with inputs from empirical testing. A period of slow increase in temperature called the TD induction period is usually present. This induction period typically end at a point (the run-away point) when the rate of increase of temperature**

Technical Paper On NC thermal decomposition Mario Paquet Page 2 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc accelerate rapidly to the ignition point. The ignition temperature (Tign) is essentially the temperature at which the decomposition is self-sustaining. Below that temperature; the decomposition may be stopped by lowering the temperature. However, during a time period just prior to ignition which is identified as the run-away decomposition period; the temperature may be increasing very quickly and it may be very difficult to reverse the process.

The following graphs summarize the TD type: Figure 1 Figure 2 For TD type of material of a given mass and shape; below the Tc, the mass is not self-heating and decomposition is according to Arrhenius relation; it is slow enough that there is no appreciable increase in temperature. When the isothermal temperature is at or above the Tc, an induction period is usually present. The induction periods gets shorter as the isothermal set-point increases above Tc.

At very high isothermal set-points, the TD induction period may be so short as to essentially disappear and the decomposition jumps directly to runaway condition and ignition. In that case, ignition is at the surface of the material and it becomes essentially independent of size and shape. The fast-event ignition threshold is an important point in the decomposition curve. Below the fast-event ignition threshold; Tc is dependent on the size or the shape of the sample and TD is dependent on temperature, size and shape. The ignition is expected to occur from the center of the mass where temperature is the highest.

The run-away decomposition period is typically very short relative to the TD induction period and the run-away temperature (T)RA is often taken to be the temperature of ignition (Tign) or somewhere in between. The Autocatalitic (AC) group Chemicals from the Autocatalytic (AC) group, when subjected to isothermal conditions, will quickly warm up to the isothermal set-point and will not continue to self-heat significantly above that temperature like a TD chemical. However, some decomposition of the chemical will slowly generate an autocatalyst at a rate following an Arrhenius equation depending on thermal history and thermal conditions.

The concentration in autocatalyst will gradually increase during the AC induction time period. Above a certain threshold in autocatalyst concentration, the self-heating decomposition reaction will start. At this point, the material will behave like a TD chemical and may go through a TD induction period if temperature is above Tc. The AC induction period is temperature specific and does not depend on the size or shape of sample. However, the TD induction period is temperature specific and depends on the size and shape of sample as stated previously. NC and NG are members of that group.

Technical Paper On NC thermal decomposition Mario Paquet Page 3 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Figure 3 One important characteristic is the Time to Self Accelerating Decomposition or TSAD. The TSAD is specific to a given isothermal set-point; there is therefore as many TSAD as there are possible isothermal set-point for NC samples. A soon as NC has completed its stabilization process in an NC plant, its start degrading. However when NC samples are stored at temperatures below 30°C, the effect of aging is negligible (typically the AC induction time for NC is greater than 10 years).

It is also possible to quantify the quality of the stabilization and also find the equivalent isothermal age of NC samples by evaluating the TSAD under given isothermal condition.

For a standard arbitrary TSAD of 7 days or 10080 minutes; the related temperature is identified in most publications as the SADT or Self Accelerating Decomposition Temperature. This specific SADT in this paper is termed the Standard SADT. The Standard SADT determination is usually established by an isothermal storage test. The Standard SADT is useful to give a relative rating of the sensitivity of various explosives to aging in storage. The following abbreviations for the present paper have been adopted: For isothermal conditions: -SADT@T°C is the Self-Accelerating Decomposition Temperature at a given temperature T°C for under isothermal conditions.

-TSAD@T°C is the Time to Self-Accelerating Decomposition Temperature at a given temperature T°C for under isothermal conditions and is directly associated to the SADT@T°C. For non-isothermal conditions: -TSADnon-isothermal and SADTnon-isothermal must be provided with the actual non-isothermal conditions they are related to. The TSAD is important because prior to it; the decomposition is theoretically independent of the sample size and shape and the AC induction time is basically driven only by the concentration in autocatalyst and the isothermal condition. Note: This previous statement is not entirely accurate since the time to equilibrate to the isothermal conditions is obviously affected by the shape and size of samples and also the detection of the beginning of the self-heating phase may be more precisely ascertained for larger samples which may produce larger signal for detection.

**However, these variables may be made insignificant for longer AC induction period. A minimum amount of material must be available to affect a thermal increase by self-heating and therefore analytical procedures using more NC have a better ability to detect the transition from the AC induction period to the DT induction period.**

Technical Paper On NC thermal decomposition Mario Paquet Page 4 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc For NC, the TSAD enable the quantification of the aging effect various temperatures under both isothermal and non- isothermal conditions. When the auto catalyst concentration reaches a critical concentration; the self-heating phase begins if the constant temperature is above the critical temperature. From that point on; the increase in temperature will be dependent on the sample size and shape in addition to isothermal condition.

Figure 4 At very high isothermal set-points, the induction periods (AC and TD) may be so short that it, in effect, disappears and the decomposition proceed directly to the runaway condition and to ignition. In that case, the ignition is at the surface of the material and it becomes essentially independent of size and shape. The fast-event ignition threshold is an important point in the decomposition curve. Below the critical temperature (Tc) of the TD phase; the sample will be in a metastable state where the material is stable as long as it is kept below the critical temperature. If the sample is brought to a temperature above the critical temperature; it will start self-heating at a rate dependent on the size, shape, isothermal set-point and concentration of auto-catalyst.

If the level of decomposition is very advanced above the critical concentration; self-heating may be fast enough as to be essentially instantaneous.

Therefore, a sample of the AC type may be in various state of stability depending on its thermal history: -Stable: samples which are still in the AC induction period -Unstable: samples with no AC induction period left and in the TD induction period and kept at temperature above the Tc -Metastable: samples with no AC induction period left and in the TD induction period and kept at temperature below the Tc Metastable samples are in a precarious state of stability; a sudden change in temperature (bringing the temperature above the Tc) may be sufficient for ignition with all the consequences that this may imply.

It is important to quantitatively know the state of decomposition of a sample in order to properly assess the risk of a situation when confronted by an abnormal sample and select the safest mean of eliminating the threat.

2 Building the empirical decomposition curve for NC Decomposition of NC: slow events

Technical Paper On NC thermal decomposition Mario Paquet Page 5 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc The work by Takashi Kotoyori published in 2008 on “Critical temperature for the thermal explosion of chemicals” reviews the basic concepts of TD and AC decomposition of chemicals and it provides some very valuable information about NC decomposition under isothermal conditions. The time to self-accelerated decomposition of NC is provided for a range of 1 to 10 days.

To this can be added the data presented by Turcotte and all which tested NC under isothermal conditions using ARC in air covering a range of 5 hrs to 1 day. Both used about 0.5g samples confined in closed cell and under isothermal condition for estimating the end of the autocatalytic phase and the beginning of the self-accelerated decomposition phase: this is important as NC is typically stored in sealed drums or boxes. Decomposition of NC is significantly affected by confinement especially in isothermal mode. Both set of data are presented in the following Arrhenius type plot: Figure 5 The values of Ea (unit kJ mol-1) and ln A (unit min-1) are obtained from the Arrhenius type plots for the data points from Turcotte and all (Arrhenius1) and Tokoyori (Arrhenius2).

The Activation Energy (Ea) is the slope divided by gas constant (R) and the Pre-exponential Factor also called the Frequency Factor (ln A) is the y-intercept. Decomposition of NC: fast events The work done by A.S Shteinberg published in 2010 (translated from Russian) on fast reactions of energetic materials provides precious data about the fast thermal decomposition of NC. The samples were dry pellets of NC with a density near 1.5g/cc (nitrogen content of about 13.50%). The pellets were 12mm (blue circle in following graphs) and 18mm (red circle in following graphs) in diameter and about 6 mm long.

The initial NC temperature is about 23°C ±2.5°C: Figure 6 Figure 7 Constructing the empirical TSAD curve for NC The 3 groups of data from Tokoyori, Turcotte and all and Shteinberg are combined in the following graph. It is important to remember that the set of data from Shteinberg on fast events ignition represent the actual time to ignition while the data

Technical Paper On NC thermal decomposition Mario Paquet Page 6 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc from Kotoyori and Turcotte and represent the time to self-accelerated decomposition (TSAD). A sigmoidal Margin-Mercer and Flourin (MMF) regression is fitted through the data as a reference. The MMF curve is asymptotic below about 60°C and is not plotted further on. Figure 8 The sections above 7 days and between 2 minutes and 4 hrs are still to be completed and further testing is underway. For long term storage of NC; information below about 60 minutes is not important.

The section above 60 minutes is of interest and can be divided 2 two sub-sections: the testing range and the storage range. The testing range is between 60 minutes and 10 hrs. Both the Methy Violet Paper (MVP) stability heat test at 134.5°C and the Bergan-Junk stability heat test at 132°C are in that range. The storage range is above 24 hrs and is usually measured in days, months or years. Two Arrhenius equations can be used to estimate the TSAD (time to self-accelerated decomposition) at a given isothermal set-point following the general relationship: Eq 1 TSAD@T°C = EXP ( Ea / R * 1000 / (T°C + 273.15) – A ) For TSAD greater than about 14 hrs (or 840 minutes) or temperature lower than about 95°C, the Arrhenius1 equation is used: Eq 2 TSAD@T°C = EXP ( 137.0 / 8.31441 * 1000 / (T°C + 273.15) - 38.0 ) Or TSAD@T°C = EXP ( 16477 / (T°C + 273.15) - 38.0 ) For TSAD between 6 minutes and 14 hrs (or 840 minutes) or temperature between 95°C and 190°C, the Arrhenius2 equation is used: Eq 3 TSAD@T°C = EXP ( 75.6 / 8.31441 * 1000 / (T°C + 273.15) - 17.9 ) Or TSAD@T°C = EXP ( 9092.6 / (T°C +273.15) – 17.9 )

Technical Paper On NC thermal decomposition Mario Paquet Page 7 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc In addition a sigmoidal model was used (Harris equation) to plot a curve through the data points along both Arrhenius plots in the range of main interest. Using this relation; the time in minutes to the self-accelerated decomposition under isothermal conditions or TSAD@T°C can be estimated between 10 minutes and 19 yrs and between 30°C and 170°C . This curve cannot be used for temperatures below 30°C as it does not follow the Arrhenius1 relation in that region.

In the range from 30°C to 170°C; the model reproduces the data points within about ±2°C: Eq 4 TSAD@T°C ( ( 1-(A*T°C))/(T°C*B))^(1/C)) Or conversely: T°C = (1/(A+(B*( TSAD@T°C ^C)))) Where: T°C = Temperature °C A = -0.00140492 B = 0.00591459 C = 0.09974258 Figure 9 Around 14 hrs (or 95°C); the empirical decomposition curve diverge from the Arrhenius1 decomposition curve and follows the Arrhenius2 decomposition curve, which follow the Harris model. At temperature higher than 95°C, the decomposition takes more time then what is predicted by the Arrhenius1 equation and follows the Arrhenius2 decomposition curve.

It is assumed that because there is enough energy to sponsor other reactions, the end of the autocatalysis phase is delayed. Below about 6 minutes; temperature is getting near the actual ignition temperature of NC and the time it takes to achieve ignition is mainly governed by the time it takes to heat-up the sample to ignition temperature. This would put the ignition temperature somewhere between 200 and 220°C.

Thus the decomposition of NC under various isothermal conditions can be divided in 3 groups: -Fast decomposition: events < 6 minute or at temperature above 190°C -Slow decomposition: events > 14 hrs or at temperature below 95°C -Mid-range decompositions: events between 6 minute and 14 hrs or at temperature between 95 and 190°C The curve is strongly dependent on the quality of stabilization of the NC and sometimes there are significant variations between lots and manufacturers of NC. The data is obtained from dry, high nitrogen NC. The typical variations for

Technical Paper On NC thermal decomposition Mario Paquet Page 8 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc recently stabilized NC lots tested using MVP stability test typically extend on a range of about ±15% of the average which is plotted on the following graph: Figure 10 About the TD phase of the NC decomposition The mid-range decomposition zone and slow decomposition zone is the TSAD (time to self-accelerated decomposition) while the fast decomposition zone is the time to ignition.

To make the graph complete; the time to ignition curve should be added. At this time: data to produce this red curve is not available and no computation has been done. This curve is affected by the size and shape of the samples and would be estimated using the Frank-Kamenetskii equations with inputs from empirical testing. The distance between the blue and red curves would be equivalent to the TD induction period. As expected it should be shorter at higher temperature. At lower temperatures, the curve become asymptotic and the TD induction times increase to infinity: this would be the TD Critical Temperature (Tc) of the curve.

Below that value; NC would be in a metastable state.

Figure 11

Technical Paper On NC thermal decomposition Mario Paquet Page 9 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc This aspect of the decomposition will not be address further by this paper. For safety purpose: the conservative approach is to consider unsafe any NC in storage that gets close to the end of the AC induction time period. 3 Using the stability test data to evaluate the various shelf-lives of NC The main method of evaluation of stability is the Methyl Violet Paper test (MVP) and the Bergmann-Junk test (BJ).

Both tests detect the amount of NO2 produced during heating under isothermal condition. Above a definite quantity of NO2, the test will fail and the material will be deemed not sufficiently stable to be used in most applications. However, it does not make any statement about how safe a material is and how long can it can be kept in storage until remediation measures for restabilization or disposition are available.

A specific concentration of NO2 will define the end-point of the MVP and BJ stability tests. The concentration in NO2 is not exactly the same for both tests which are done at two different isothermal temperatures. Table 1: Basic test conditions for MVP and BJ stability heat test Test Isothermal Temperature Weight (g) Time to end-point (minutes) Estimated TSAD at test temperature MVP 134.5°C 2.5 Typically 35 82.5 minutes BJ 132°C 2.0 Fix 120 94.7 minutes The MVP test will be completed early in the AC induction period while the BJ test will consume all of the AC induction period and some of the TD induction period.

This paper will focus on MVP stability heat test to evaluate the 2 shelf-lives of NC: the time to stability test failure and the time it will take for NC to become a safety hazard in storage. Note: In term of safety, the MVP stability heat test is more forgiving then the BJ stability test when testing low stability NC samples. The MVP stability heat test safety factor is about 2X since it last at most about 35-40 minutes and the TSAD at 134.5°C is about 82.5 minutes or twice the time of the test. The MVP heat test is completed before reaching the SAD (self-accelerated decomposition). The BJ test requires sample to be heated beyond the expected SAD point into the TD induction phase where more NO2 is produced.

When testing NC samples of unknown stability, or suspected of being degraded: the MVP test as a definite advantage over the BJ test. On the other hand, it should also be remembered that in the BJ test a significant amount of NO2 is extracted by the trapping solution; reducing the content in NO2 in the test tube and affecting the AC induction phase by somewhat prolonging it. It is unknown at this time by how much. The amount of degradation when testing NC using the MVP stability can be appreciated by monitoring the % weight lost over time. Several samples of Grade B (nitrogen content about 13.55%) were tested at 134.5°C and the results obtained summarized in the following graph:

Technical Paper On NC thermal decomposition Mario Paquet Page 10 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Figure 12 The degradation is significant in term of weight lost. The transition between the AC phase and TD phase is expected to occur after a degradation of about 3.5-4.5% of the mass of NC. For a MVP test to be successful; the weight loss at the end of the test should be below about 0.8% (note: precision weighing is now rapid, low-cost and traceable to national standards, therefore it provides another way of verifying NC stability).

This represents a very large quantity of gaseous NO2. This can be seen in the following pictures taken using freshly stabilized Grade B NC with nitrogen content near 13.55% and previously tested at 35±1 minutes using MVP test. The AC induction period at 134.5°C is expected to end after about 83 minutes: Figure 13 In consequence, NC in storage can easily be evaluated by the presence of NO2 fumes in the headspace above the NC in the drums. NC is usually stored in drums or boxes using clear plastic bags to preserve the NC’s water content. The absence of red gaseous NO2 in the headspace is a visible indication that the NC is still early in the AC induction phase (less than about 30% of the AC induction period).

Using the MVP test to evaluate the shelf-lives of NC

Technical Paper On NC thermal decomposition Mario Paquet Page 11 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Based on the TSAD empirical curve, the TSAD (time to self-accelerated decomposition) for a properly stabilized NC sample kept in isothermal condition at 134.5°C is about 82.5 minutes (TSAD@134.5°C = 82.5 minutes). The Methyl Violet Paper stability test (MVP test) is done at 134.5°C and the typical variations in stability of NC samples is between 25 minutes and 45 minutes with an average of about 35 minutes ( tMVP ref = 35 minutes) for most freshly stabilized samples of NC grade B (near 13.50% nitrogen) and NC grade C1 (near 13.15% nitrogen and composed of about 66% of NC Grade B at about 13.45% nitrogen).

Figure 14 Thus for the MVP stability heat test: The test is performed on 2.5 g of NC according to the standard procedure and heat testing conditions are maintained until the test paper reaches its salmon-pink end-point. According to Mil-DTL-244C; the minimum time required for a NC sample to pass the MVP test is 25 minutes at which time, some coloration must be left on the indicator paper and the test in then recorded at 30 minutes. When monitoring NC in storage at GD-Valleyfield; the test tube is inspected about every 5-10 minutes from the beginning of the test (for safety reason) and the indicator paper is inspected every 2 minutes from the 25 minutes mark.

The time it takes for the test paper to reaches its end-point (point of last discoloration) is reported with a precision of ±2 minutes. The time to test paper end-point is noted (tMVP).

Thus: tMVP = Time to indicator paper end-point of a sample of NC under investigation TSAD@134.5°C = TSAD of fresh NC -about 82.5 minutes tMVP ref = Average time to indicator paper end-point for a fresh NC sample -35 minutes TSAD@T°C = TSAD of fresh NC at any selected Temperature (T°C) in minutes The estimated time spent in storage relative to the total AC induction period is obtained from isothermal testing at 134.5°C and is expressed as %tin storage@134.5°C: Eq 5 %tin storage@134.5°C = ( tMVP ref - tMVP ) X 100 / TSAD@134.5°C = ( 35 minutes - tMVP ) X 100 / 82.5 minutes The estimated time spent in storage at other isothermal storage Temperature (T°C): Eq 6 tin storage@T°C = %tin storage@134.5°C / 100 X TSAD@T°C

Technical Paper On NC thermal decomposition Mario Paquet Page 12 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc The estimated remaining storage time before self-accelerated decomposition (tremaining storage@T°C) at other isothermal storage Temperature (T°C): Eq 7 tremaining storage@T°C = ( 100 - %tin storage@134.5°C ) / 100 X TSAD@T°C For example: -A NC sample with a MVP test at 26 minutes (tMVP = 26) has spent in storage 10.9% of the total AC induction (% tin storage@134.5°C = 10.9%). This means that about 11% of the time necessary to start the self-heating decomposition has been depleted.

Calculation: % tin storage@134.5°C = ( tMVP ref - tMVP ) X 100 / TSAD@134.5°C = ( 35 – 26 ) x 100 / 82.5 = 10.9%. For example: -In storage under isothermal condition at 33°C; a freshly made sample of NC with a MVP result of about 35 minutes (TSAD@134.5°C = 35) has a TSAD of about 19.0 years (TSAD@33°C = 19.0yrs). A NC sample with a MVP test at 26 minutes (TSAD@134.5°C = 26) is expected to have its TSAD reduced to about 17.0 yrs (tremaining storage@33°C = 16.9yrs) or a reduction in storage time of about 2.1yr.

For example: -In storage under isothermal condition at 46°C; a freshly made sample of NC with a MVP result of about 35 minutes (TSAD@134.5°C = 35) has a TSAD of about 23 months (TSAD@46°C = 23months). A NC sample with a MVP test at 26 minutes (TSAD@134.5°C = 26) has spent in storage 10.9% of the total AC induction (% tin storage@134.5°C = 10.9%) is expected to have its TSAD reduced to about 20.5 months (tremaining storage@46°C = 20.5 months) or a reduction in storage time of about 2.5 months.

For example: -In storage under isothermal condition at 60°C; a freshly made sample of NC with a MVP result of about 35 minutes (TSAD@134.5°C = 35) has a TSAD of about 6 weeks (TSAD@60°C = 6 weeks).

A NC sample with a MVP test at 26 minutes (TSAD@134.5°C = 26) and a lost in stability of 10.9% (%tin storage@134.5°C = 10.9%) is expected to have its TSAD reduced to about 5.3 weeks (tremaining storage@60°C = 5.3 weeks) or a reduction in time of about 0.7 week. If the time to the test paper end-point (tMVP) is greater than 35 minutes than: The %tin storage@134.5°C and tin storage@T°C will be negative meaning the NC has extra storage time and the tremaining storage@T°C will be greater than the TSAD@T°C because of the extra storage time.

4 Dealing with non-isothermal testing or storage conditions: Temperature ramps are often encountered in NC thermal test and increases the complexity of data analysis. It is possible to estimate the effect of non-isothermal testing on TSADnonisothermal and SADTnonisothermal for NC. Knowing the isothermal empirical decomposition curve for NC allows dealing with the non-isothermal conditions through numerical analysis by assuming a quasi-static process. The non-isothermal event can be subdivided in equal portion of time each with a given temperature. For each time interval of a given temperature T°C, the TSAD@T°C is calculated using one of the empirical equations.

Then the % contribution to decomposition is calculated by dividing the time interval by the TSAD@T°C. All the % contribution are added and when the total is equal to 100%, the TSADnon-isothermal (time to self-accelerated decomposition non-isothermal) is obtained and SADTnon-isothermal (self-accelerated decomposition temperature non-isothermal). Both are specific to the thermal conditions followed during the test.

Technical Paper On NC thermal decomposition Mario Paquet Page 13 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Example: When will a NC sample start self-heating and at what temperature if it is exposed to a temperature ramp starting at 25°C and increasing at a rate of 5.7°C per hour? The TSADnon-isothermal and SADTnon-isothermal need be estimated. Summary of calculations for the following worksheet: -a linear increase in temperature of 5.7°C/hr or 0.095°C/min - a starting temperature of 25°C -the steps are arbitrarily set to 2979 sec (here adjusted to fit the table provided below and to get one of the summations of decomposition contribution as close as possible to 100.0%, however usually the time interval is reduced until convergence is obtained) -since the temperature is expected to cover a range between 25°C and more than 100°C, the combined sigmoidal model (Harris equation) is selected (Eq 4): TSAD@T°C ( ( 1-(-0.00140492*T°C))/(T°C*0.00591459))^(1/0.09974258)) -the %contribution to decomposition is calculated for each step: % contribution to decomposition = TSAD@T°C x 100 / Step/min -the summation of actual and previous %contribution is calculated for each step -The TSADnon-isothermal and SADTnon-isothermal is obtained when the summation reach 100% Worksheet describing the calculation: Figure 15 Here the summation of decomposition contribution reaches 100% when TSADnon-isothermal = 16.6 hrs and SADTnon-isothermal = 119.4°C.

Other example: When will a NC sample start self-heating and at what temperature if it is exposed to a temperature ramp starting at 25°C and increasing at a rate of 17.0°C per hour?

Technical Paper On NC thermal decomposition Mario Paquet Page 14 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Here the summation of decomposition contribution reach 99.9% when TSADnon-isothermal = 6.4 hrs and SADTnon-isothermal = 133.6°C. Using this or similar approaches; decomposition temperature and time to self-accelerated decomposition for non- isothermal conditions can be estimated.

The average reduction in storage time per year (expressed as % of TSAD) for a given facility Most NC storage facilities do not store under isothermal conditions. It is possible to evaluate the average reduction in storage time per year (expressed as % of TSAD) for a given facility. For this, the temperature variation, ideally for every hour, for a period of 1 year minimum is required. As it will be demonstrated, every hour spent above 30°C is important and the temperature base on an average does not convey all the effect. The temperature average for Montreal, Canada for 2011 is about 7.8°C and the average for the last 20 years is about 6.2°C.

The temperatures are taken in a well- ventilated area and in the shade.

Typically for Montreal; the temperature is below 20°C for about 80% of the year and only about 0.4% of the year is above 30°C. Consequently, the average reduction in storage time per year is expected to be low. On the other hand, in an enclosed storage magazine in GD-Valleyfield, the temperature is typically about 5-7°C higher than the normally recorded temperature. Accordingly, the average reduction in storage time per year is expected to be somewhat higher. The following graphs summarize the temperature variation (in the shade) in Montreal for 2011 (total 8760hrs) and the cumulative distribution of hours for one year both normal temperature (in blue) and in storage magazine (in red): Figure 16 Figure 17 The increase by 7°C in temperature in the magazines in GD-Valleyfield cause a shifting to the right of the temperature curve and now 10% of the time per year is above 30°C instead of the previous 0.4%.

This substantial change in temperature is expected to affect considerably the NC rate of degradation. To calculate the TSAD@T°C; the Arrhenius1 equation (Eq 2) is preferred as the temperature variations are lower than 95°C and are expected to go below 20°C: TSAD@T°C = EXP ( 16477 / (T°C + 273.15) - 38.0 ) For every temperature data point; the contribution to the average reduction in storage time per year (expressed as % of TSAD) for a given facility is calculated. All the contributions are added to produce the average reduction in storage time per year (expressed as % of TSAD) for a facility near Montreal or location where the temperature variations are similar to Montreal.

Technical Paper On NC thermal decomposition Mario Paquet Page 15 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Figure 18 Figure 19 The average reduction in storage time per year (expressed as % of TSAD) is about 0.4% of the TSAD for a storage facility near Montreal in the shade and well-ventilated area. In an enclosed storage magazine in Valleyfield, the temperature is typically about 7°C higher than the normally recorded temperature and increases the average reduction in storage time per year to about 1.4% of the TSAD.

As expected the summer months (between 4000 and 6000 hrs) contribute the most. Estimating the time to failure of MVP test and time to self-accelerated decomposition in storage Since the total TSAD is 100%, than 100% / 1.4% = about 71 years of storage time before reaching the end of the AC induction period and for NC to start self-accelerated decomposition. A fresh NC with a MVP near 35 minutes will have a maximum storage time of about 11% of the total TSAD; so 11% / 1.4% = about 7.8 years of storage before failure of the MVP test. This value is substantiated by the typical storage time before failure of the MVP in GD-Valleyfield (about 7 to 9 yrs).

Example: -What is the estimated time to MVP stability test failure for a NC sample with a MVP test result of 32 minutes? A NC sample with a MVP test at 32 minutes (tMVP = 32) exhibit a loss in stability of 3.6% (% tin storage@134.5°C = 3.6%) or % tin storage@134.5°C = ( tMVP ref - tMVP ) X 100 / TSAD@134.5°C = ( 35 – 32 ) x 100 / 82.5 = 3.6%. The failure of the MVP (end-point shorter than 26 minutes) occurs at 11% of the TSAD. The average reduction in %TSAD per year in typical storage conditions near Montreal is about 1.4% per year. Thus (11%-3.6%) / 1.4% per yr = about 5.3 years before failing the MVP stability test.

-How old is the sample? Assuming an original MVP of 35 minutes: the % tin storage@134.5°C is about 3.6% and the average reduction in %TSAD per year is 1.4%, then 3.6% / 1.4% = about 2.6 yrs old (note: if the actual original MVP result is known for the sample, a more precise evaluation can be done). -What is the estimated time to self-accelerated decomposition (end of AC phase) for that sample? The average reduction in %TSAD per year in typical storage conditions near Montreal is about 1.4%/per year. Thus (100% - 3.6%) / 1.4% per yr = about 69 years before starting the self-accelerated decomposition phase.

A closer look at the contribution of various temperatures to the average reduction in storage time per year (expressed as % of TSAD) for NC stored in Valleyfield; the time spent at temperatures below 23°C account for less than about 10% of the average reduction per year of storage time although it represent more than 65% of the annual hours. While the temperatures above 30°C account for more than 50% of the average reduction per year of storage time although this

Technical Paper On NC thermal decomposition Mario Paquet Page 16 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc represent less than 10% of the annual hours. Therefore any increases in temperatures above 20°C are meaningful and above 30°C are important. Estimating shelf-lives in storage in other locations Obviously, Montreal has a rather low yearly average temperature. Other locations with higher yearly average temperature will have to adjust the storage requirements accordingly. These higher storage temperatures will considerably affect the storage limit for NC.

The average reduction in storage time per year (expressed as % of TSAD) for NC can be estimated from specific annual temperature data for a given area or location.

Based on the typical variations relative to the yearly average temperature, the following graph provides a rough estimate of the average reduction in storage time per year (expressed as % of TSAD). To the yearly average temperature for a given area should be added the temperature increase due to storage conditions at the facility. Typical yearly average temperature for different locations are available in the following table and approximated average reduction is storage time (expressed as % of TSAD) for NC (high nitrogen content) relative to the yearly average temperature can be obtained from the following graph: Table 2 Figure 20 In the previous graph, above a yearly average temperature of about 30-35°C; the average reduction in storage time come to be so large that decomposition is not multi-years anymore: decomposition may occur in 1 or 2 summer seasons.

Storage under those temperature conditions is extremely difficult and implies extra safety concerns. It is possible to estimate typical shelf-life to MVP test failure (assuming a certain starting MVP result) and the shelf-life marked by the ending of the AC induction period and the beginning of the self-accelerated temperature increase. From the AC self-life can be estimated a safety shelf-life for storage of NC by setting a safety margin based on local practice and standards. The following tabulates these approximations:

Technical Paper On NC thermal decomposition Mario Paquet Page 17 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc Table 3 Obviously, this is a rule of thumb and wide safety margins are recommended when using such a general approach. It is recommended to verify and establish safety guidelines after careful evaluation, proper temperature measurements and applying large safety margins. It must always be remembered that drums can be lost or forgotten. NC in storage is subject to very diverse storage conditions (near a wall with sunlight –radiance, high variations in water content within a drum in storage, …) and analysis is always performed on a small sample of the population.

This always assumes storage in the shade with no direct sunlight at any time on the drums. Exposition to direct sunlight (through doors or windows) can significantly reduce the self-life of NC in storage.

Example: Exposed to the sun during the summer at GD-Valleyfield, a drum surface temperature will easily reach a temperature of about 65-70°C. Typically, direct contact of the drum surface with the skin will produce severe burn in about 2-3 seconds. In those conditions, the average reduction in %TSAD per hour (not year) is about 0.34%, therefore the NC in the drum will fail the MVP stability test after about 30hrs of exposition; assuming a direct exposition of about 8 hrs per day: about 4 days. It will start the self-accelerated decomposition after about 300 hrs of direct exposition in the sun; assuming a direct exposition of about 8 hrs per day: the drum will start it TD phase in about 37 days or about 1 month.

In GD-Valleyfield all NC lots are added to the stability surveillance program after 2 years of manufacturing (tested every year from that moment). All lots are tested just before use and no NC is stored for more than 10 years. Most NC will failed MVP test after about 7 to 9 years in storage except for lots with initial low MVP results (lower stabilization quality). One other important point is NC facilities which manufacture and sell NC cannot follow the minimum requirement set by the MIL-DTL-244C if the NC is to be transported and stored a certain period of time prior to utilization. A certain buffer should exist in order to allow for a reasonable time period between lot certification and consumption especially if the user is located in an area with a high yearly average temperature.

Typically, appropriately stabilized NC coming out of a NC facility should have a MVP test result near about 35 minutes in order to provide the user time to receive and process the NC. Facilities where the NC plant is directly attached to the propellant facility do not necessarily need such a large buffer. 5 Conclusions The methodology presented here should be taken as a rule of thumb. Since the empirical curve is exponential and covers more than 9 orders of magnitude, the precision is low and large safety margin should be applied. More data point are required to better detailed the empirical curve and the effect of moisture content, and pressure should be investigated.

It is important to take into consideration the historical evidences from existing facilities in order to confirm that the estimates and possible guidelines are based on solid ground.

Technical Paper On NC thermal decomposition Mario Paquet Page 18 / 18 March, 2012 D:\20120131 NC Symposium Spiez\20120221 NC Symposium Paper GD Valleyfield Thermal decomposition Final.doc It is clear that the exact description and calculation of a specific case of thermal aging of NC in storage is to all intents and purposes very difficult since those are exceedingly intricate events. However, it is possible to generate some numerical data that will permit a semi-quantitative evaluation of the relative safety and produce the basic information necessary for the proper establishment of the basis of safety.

The results obtain from these simulations are crude estimate of what can actually happened in storage over long period of time. The results obtain from this work are useful only in that they may help better understand the various aspect of NC in storage and analysis of data from stability testing. References [1] Nitrocellulose Specification MIL-DTL-244 Revision C Detail specification for nitrocellulose approved for use by all departments and agencies of the US Department of Defense. Project Manager for Combat Ammunition System, Picatinny Arsenal, N.J. 07806-5000.

[2] NATO Standardisation Agreement (NATO STANAG) 4178, edition 2. Test procedures for assessing the quality of deliveries of nitrocellulose from one NATO nation to another. Military Agency for Standardisation, NATO Headquarters, Blvd Leopold III, 1110 Brussels, Belgium. [3] T.Kotoyori. Critical temperature for thermal explosion of chemicals Industrial Safety Series, Volume 7, Elsevier (2005) 303-338 [4] A.S.Shteinberg Fast reactions in energetic material (translated from Russian) Springer (2006) 80-83 119-122 [5] R. Turcotte, B. Acheson, S. Singh and M. Paquet Effect of Pressure on the Thermal Decomposition of Nitrocellulose and its Mixtures with Nitroglycerin CANMET Canadian Explosives Research Laboratory Report (2006)